#------------------------------------------------------------------------------
#$Date: 2017-04-13 05:19:17 +0300 (Thu, 13 Apr 2017) $
#$Revision: 195403 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/04/26/7042689.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7042689
loop_
_publ_author_name
'Peschke, Simon'
'Gamperl, Lisa'
'Weippert, Valentin'
'Johrendt, Dirk'
_publ_section_title
;
 Flux Synthesis, Crystal Structures, and Physical Properties of New
 Lanthanum Vanadium Oxyselenides
;
_journal_name_full               'Dalton Trans.'
_journal_paper_doi               10.1039/C7DT00779E
_journal_year                    2017
_chemical_formula_sum            'La7 O7 Se5 V'
_chemical_formula_weight         1530.1
_chemical_name_systematic
;
 ?
;
_space_group_crystal_system      orthorhombic
_space_group_IT_number           63
_space_group_name_Hall           '-C 2c 2'
_space_group_name_H-M_alt        'C m c m'
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_audit_creation_method           SHELXL-2014
_audit_update_record
;
2017-03-02 deposited with the CCDC.
2017-03-31 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   3.9859(2)
_cell_length_b                   12.8627(5)
_cell_length_c                   32.2904(14)
_cell_measurement_reflns_used    2020
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      24.996
_cell_measurement_theta_min      3.235
_cell_volume                     1655.51(13)
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.969
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Bruker CCD'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0475
_diffrn_reflns_av_unetI/netI     0.0309
_diffrn_reflns_Laue_measured_fraction_full 0.969
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       4
_diffrn_reflns_limit_h_min       -4
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       38
_diffrn_reflns_limit_l_min       -38
_diffrn_reflns_number            6698
_diffrn_reflns_point_group_measured_fraction_full 0.969
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         24.996
_diffrn_reflns_theta_min         1.261
_exptl_absorpt_coefficient_mu    29.182
_exptl_absorpt_correction_T_max  0.7465
_exptl_absorpt_correction_T_min  0.5705
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    6.139
_exptl_crystal_description       needle
_exptl_crystal_F_000             1296
_exptl_crystal_size_max          0.04
_exptl_crystal_size_mid          0.005
_exptl_crystal_size_min          0.005
_refine_diff_density_max         1.770
_refine_diff_density_min         -1.971
_refine_diff_density_rms         0.401
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.132
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     54
_refine_ls_number_reflns         854
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.132
_refine_ls_R_factor_all          0.0373
_refine_ls_R_factor_gt           0.0321
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0339P)²+80.4217P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0740
_refine_ls_wR_factor_ref         0.0793
_reflns_Friedel_coverage         0.000
_reflns_number_gt                769
_reflns_number_total             854
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c7dt00779e2.cif
_cod_data_source_block           shelxl
_cod_original_formula_sum        'La7 O7 Se5 V1'
_cod_database_code               7042689
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelxl_version_number           2014-3
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z+1/2'
'-x, y, -z+1/2'
'x, -y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z'
'-x, -y, -z'
'x, y, -z-1/2'
'x, -y, z-1/2'
'-x, y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, y+1/2, -z-1/2'
'x+1/2, -y+1/2, z-1/2'
'-x+1/2, y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
La1 La 0.0000 0.05799(9) 0.2500 0.0071(3) Uani 1 4 d S T P
La2 La 0.5000 0.86554(7) 0.31307(2) 0.0073(2) Uani 1 2 d S T P
La3 La 0.0000 0.03585(7) 0.38615(2) 0.0076(2) Uani 1 2 d S T P
La4 La 0.5000 0.82050(7) 0.43722(2) 0.0078(2) Uani 1 2 d S T P
Se1 Se 0.0000 0.72405(12) 0.36802(4) 0.0103(4) Uani 1 2 d S T P
Se2 Se 0.5000 0.24682(17) 0.2500 0.0098(5) Uani 1 4 d S T P
Se3 Se 0.5000 0.87873(12) 0.53020(4) 0.0103(4) Uani 1 2 d S T P
V1 V 0.0000 0.0000 0.5000 0.0087(8) Uani 1 4 d S T P
O1 O 0.5000 0.9654(10) 0.2500 0.003(3) Uiso 1 4 d S . P
O2 O 0.0000 0.0824(8) 0.5511(3) 0.006(2) Uiso 1 2 d S . P
O3 O 0.5000 0.9394(8) 0.3823(3) 0.008(2) Uiso 1 2 d S . P
O4 O 0.0000 0.9763(8) 0.3171(3) 0.009(2) Uiso 1 2 d S . P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
La La -0.2871 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 La1 O1 118.3(6) 1_445 1_545
O1 La1 O4 77.07(16) 1_445 10_546
O1 La1 O4 77.07(16) 1_545 10_546
O1 La1 O4 77.07(16) 1_445 1_545
O1 La1 O4 77.07(16) 1_545 1_545
O4 La1 O4 128.3(5) 10_546 1_545
O1 La1 Se2 81.5(3) 1_445 1_455
O1 La1 Se2 160.2(3) 1_545 1_455
O4 La1 Se2 109.71(18) 10_546 1_455
O4 La1 Se2 109.71(18) 1_545 1_455
O1 La1 Se2 160.2(3) 1_445 .
O1 La1 Se2 81.5(3) 1_545 .
O4 La1 Se2 109.71(18) 10_546 .
O4 La1 Se2 109.71(18) 1_545 .
Se2 La1 Se2 78.74(6) 1_455 .
O1 La1 La2 37.85(13) 1_445 10_446
O1 La1 La2 96.7(2) 1_545 10_446
O4 La1 La2 39.50(13) 10_546 10_446
O4 La1 La2 101.5(2) 1_545 10_446
Se2 La1 La2 99.91(2) 1_455 10_446
Se2 La1 La2 147.342(13) . 10_446
O1 La1 La2 37.85(13) 1_445 1_445
O1 La1 La2 96.7(2) 1_545 1_445
O4 La1 La2 101.5(2) 10_546 1_445
O4 La1 La2 39.50(13) 1_545 1_445
Se2 La1 La2 99.91(2) 1_455 1_445
Se2 La1 La2 147.342(13) . 1_445
La2 La1 La2 65.31(3) 10_446 1_445
O1 La1 La2 96.7(2) 1_445 10_546
O1 La1 La2 37.85(13) 1_545 10_546
O4 La1 La2 39.50(13) 10_546 10_546
O4 La1 La2 101.5(2) 1_545 10_546
Se2 La1 La2 147.342(13) 1_455 10_546
Se2 La1 La2 99.91(2) . 10_546
La2 La1 La2 63.74(2) 10_446 10_546
La2 La1 La2 98.04(4) 1_445 10_546
O1 La1 La2 96.7(2) 1_445 1_545
O1 La1 La2 37.85(13) 1_545 1_545
O4 La1 La2 101.5(2) 10_546 1_545
O4 La1 La2 39.50(13) 1_545 1_545
Se2 La1 La2 147.342(13) 1_455 1_545
Se2 La1 La2 99.91(2) . 1_545
La2 La1 La2 98.04(4) 10_446 1_545
La2 La1 La2 63.74(2) 1_445 1_545
La2 La1 La2 65.31(3) 10_546 1_545
O1 La1 La1 149.1(3) 1_445 1_655
O1 La1 La1 30.9(3) 1_545 1_655
O4 La1 La1 90.0 10_546 1_655
O4 La1 La1 90.000(1) 1_545 1_655
Se2 La1 La1 129.37(3) 1_455 1_655
Se2 La1 La1 50.63(3) . 1_655
La2 La1 La1 121.870(10) 10_446 1_655
La2 La1 La1 121.870(10) 1_445 1_655
La2 La1 La1 58.129(10) 10_546 1_655
La2 La1 La1 58.129(10) 1_545 1_655
O1 La1 La1 30.9(3) 1_445 1_455
O1 La1 La1 149.1(3) 1_545 1_455
O4 La1 La1 90.000(1) 10_546 1_455
O4 La1 La1 90.000(1) 1_545 1_455
Se2 La1 La1 50.63(3) 1_455 1_455
Se2 La1 La1 129.37(3) . 1_455
La2 La1 La1 58.129(10) 10_446 1_455
La2 La1 La1 58.129(10) 1_445 1_455
La2 La1 La1 121.870(10) 10_546 1_455
La2 La1 La1 121.870(10) 1_545 1_455
La1 La1 La1 180.0 1_655 1_455
O1 La2 O3 124.7(4) . .
O1 La2 O4 74.6(3) . 1_655
O3 La2 O4 74.0(3) . 1_655
O1 La2 O4 74.6(3) . .
O3 La2 O4 74.0(3) . .
O4 La2 O4 108.6(4) 1_655 .
O1 La2 Se1 139.93(8) . .
O3 La2 Se1 73.42(18) . .
O4 La2 Se1 143.1(2) 1_655 .
O4 La2 Se1 78.3(2) . .
O1 La2 Se1 139.93(8) . 1_655
O3 La2 Se1 73.42(18) . 1_655
O4 La2 Se1 78.3(2) 1_655 1_655
O4 La2 Se1 143.1(2) . 1_655
Se1 La2 Se1 76.20(4) . 1_655
O1 La2 Se2 73.7(2) . 5_455
O3 La2 Se2 139.86(7) . 5_455
O4 La2 Se2 143.9(2) 1_655 5_455
O4 La2 Se2 78.9(2) . 5_455
Se1 La2 Se2 72.52(3) . 5_455
Se1 La2 Se2 117.41(5) 1_655 5_455
O1 La2 Se2 73.7(2) . 5
O3 La2 Se2 139.86(7) . 5
O4 La2 Se2 78.9(2) 1_655 5
O4 La2 Se2 143.9(2) . 5
Se1 La2 Se2 117.41(5) . 5
Se1 La2 Se2 72.52(3) 1_655 5
Se2 La2 Se2 76.12(3) 5_455 5
O1 La2 La1 36.27(12) . 1_665
O3 La2 La1 103.9(2) . 1_665
O4 La2 La1 38.6(2) 1_655 1_665
O4 La2 La1 94.4(2) . 1_665
Se1 La2 La1 172.62(3) . 1_665
Se1 La2 La1 109.886(18) 1_655 1_665
Se2 La2 La1 107.18(3) 5_455 1_665
Se2 La2 La1 69.17(4) 5 1_665
O1 La2 La1 36.27(12) . 1_565
O3 La2 La1 103.9(2) . 1_565
O4 La2 La1 94.4(2) 1_655 1_565
O4 La2 La1 38.6(2) . 1_565
Se1 La2 La1 109.886(18) . 1_565
Se1 La2 La1 172.62(3) 1_655 1_565
Se2 La2 La1 69.17(4) 5_455 1_565
Se2 La2 La1 107.18(3) 5 1_565
La1 La2 La1 63.74(2) 1_665 1_565
O1 La2 La3 102.6(2) . 1_665
O3 La2 La3 36.89(11) . 1_665
O4 La2 La3 37.2(2) 1_655 1_665
O4 La2 La3 93.4(2) . 1_665
Se1 La2 La3 107.96(3) . 1_665
Se1 La2 La3 70.05(3) 1_655 1_665
Se2 La2 La3 172.00(4) 5_455 1_665
Se2 La2 La3 109.962(19) 5 1_665
La1 La2 La3 71.275(18) 1_665 1_665
La1 La2 La3 103.58(3) 1_565 1_665
O1 La2 La3 102.6(2) . 1_565
O3 La2 La3 36.89(11) . 1_565
O4 La2 La3 93.4(2) 1_655 1_565
O4 La2 La3 37.2(2) . 1_565
Se1 La2 La3 70.05(3) . 1_565
Se1 La2 La3 107.95(3) 1_655 1_565
Se2 La2 La3 109.962(19) 5_455 1_565
Se2 La2 La3 172.00(4) 5 1_565
La1 La2 La3 103.58(3) 1_665 1_565
La1 La2 La3 71.275(18) 1_565 1_565
La3 La2 La3 63.509(19) 1_665 1_565
O3 La3 O3 115.9(4) 1_445 1_545
O3 La3 O4 77.2(3) 1_445 1_545
O3 La3 O4 77.2(3) 1_545 1_545
O3 La3 O2 74.0(2) 1_445 9_556
O3 La3 O2 74.0(2) 1_545 9_556
O4 La3 O2 124.1(3) 1_545 9_556
O3 La3 Se1 157.0(2) 1_445 5_545
O3 La3 Se1 82.0(2) 1_545 5_545
O4 La3 Se1 94.18(19) 1_545 5_545
O2 La3 Se1 127.06(14) 9_556 5_545
O3 La3 Se1 82.0(2) 1_445 5_445
O3 La3 Se1 157.0(2) 1_545 5_445
O4 La3 Se1 94.18(19) 1_545 5_445
O2 La3 Se1 127.06(14) 9_556 5_445
Se1 La3 Se1 77.33(4) 5_545 5_445
O3 La3 Se3 133.1(2) 1_445 9_666
O3 La3 Se3 74.1(2) 1_545 9_666
O4 La3 Se3 145.52(3) 1_545 9_666
O2 La3 Se3 64.88(17) 9_556 9_666
Se1 La3 Se3 63.37(3) 5_545 9_666
Se1 La3 Se3 104.88(4) 5_445 9_666
O3 La3 Se3 74.1(2) 1_445 9_566
O3 La3 Se3 133.1(2) 1_545 9_566
O4 La3 Se3 145.52(3) 1_545 9_566
O2 La3 Se3 64.88(17) 9_556 9_566
Se1 La3 Se3 104.88(4) 5_545 9_566
Se1 La3 Se3 63.37(3) 5_445 9_566
Se3 La3 Se3 68.70(3) 9_666 9_566
O3 La3 La2 38.4(2) 1_445 1_445
O3 La3 La2 96.2(2) 1_545 1_445
O4 La3 La2 38.99(14) 1_545 1_445
O2 La3 La2 98.67(19) 9_556 1_445
Se1 La3 La2 130.81(4) 5_545 1_445
Se1 La3 La2 89.76(3) 5_445 1_445
Se3 La3 La2 162.46(4) 9_666 1_445
Se3 La3 La2 111.073(18) 9_566 1_445
O3 La3 La2 96.2(2) 1_445 1_545
O3 La3 La2 38.4(2) 1_545 1_545
O4 La3 La2 38.99(13) 1_545 1_545
O2 La3 La2 98.67(19) 9_556 1_545
Se1 La3 La2 89.76(3) 5_545 1_545
Se1 La3 La2 130.81(4) 5_445 1_545
Se3 La3 La2 111.073(18) 9_666 1_545
Se3 La3 La2 162.46(4) 9_566 1_545
La2 La3 La2 63.510(19) 1_445 1_545
O3 La3 La4 36.0(2) 1_445 1_445
O3 La3 La4 94.8(2) 1_545 1_445
O4 La3 La4 100.0(2) 1_545 1_445
O2 La3 La4 38.10(12) 9_556 1_445
Se1 La3 La4 164.38(4) 5_545 1_445
Se1 La3 La4 107.82(2) 5_445 1_445
Se3 La3 La4 101.03(3) 9_666 1_445
Se3 La3 La4 66.29(3) 9_566 1_445
La2 La3 La4 64.63(2) 1_445 1_445
La2 La3 La4 97.19(3) 1_545 1_445
O3 La3 La4 94.8(2) 1_445 1_545
O3 La3 La4 36.0(2) 1_545 1_545
O4 La3 La4 100.0(2) 1_545 1_545
O2 La3 La4 38.10(11) 9_556 1_545
Se1 La3 La4 107.82(2) 5_545 1_545
Se1 La3 La4 164.38(4) 5_445 1_545
Se3 La3 La4 66.29(3) 9_666 1_545
Se3 La3 La4 101.03(3) 9_566 1_545
La2 La3 La4 97.19(3) 1_445 1_545
La2 La3 La4 64.63(2) 1_545 1_545
La4 La3 La4 63.45(2) 1_445 1_545
O3 La4 O2 77.1(3) . 9_666
O3 La4 O2 77.1(3) . 9_566
O2 La4 O2 113.6(4) 9_666 9_566
O3 La4 Se3 125.2(2) . .
O2 La4 Se3 73.7(2) 9_666 .
O2 La4 Se3 73.7(2) 9_566 .
O3 La4 Se1 74.22(19) . 1_655
O2 La4 Se1 78.2(2) 9_666 1_655
O2 La4 Se1 145.5(2) 9_566 1_655
Se3 La4 Se1 139.60(2) . 1_655
O3 La4 Se1 74.22(19) . .
O2 La4 Se1 145.5(2) 9_666 .
O2 La4 Se1 78.2(2) 9_566 .
Se3 La4 Se1 139.61(2) . .
Se1 La4 Se1 75.89(4) 1_655 .
O3 La4 Se3 136.38(13) . 13_566
O2 La4 Se3 146.5(2) 9_666 13_566
O2 La4 Se3 81.7(2) 9_566 13_566
Se3 La4 Se3 83.26(4) . 13_566
Se1 La4 Se3 106.51(4) 1_655 13_566
Se1 La4 Se3 64.28(3) . 13_566
O3 La4 Se3 136.38(13) . 13_666
O2 La4 Se3 81.7(2) 9_666 13_666
O2 La4 Se3 146.5(2) 9_566 13_666
Se3 La4 Se3 83.26(4) . 13_666
Se1 La4 Se3 64.27(3) 1_655 13_666
Se1 La4 Se3 106.51(4) . 13_666
Se3 La4 Se3 71.46(3) 13_566 13_666
O3 La4 V1 90.4(2) . 1_665
O2 La4 V1 29.2(2) 9_666 1_665
O2 La4 V1 92.2(2) 9_566 1_665
Se3 La4 V1 46.40(2) . 1_665
Se1 La4 V1 106.756(19) 1_655 1_665
Se1 La4 V1 163.25(4) . 1_665
Se3 La4 V1 128.36(3) 13_566 1_665
Se3 La4 V1 89.14(2) 13_666 1_665
O3 La4 V1 90.4(2) . 1_565
O2 La4 V1 92.2(2) 9_666 1_565
O2 La4 V1 29.2(2) 9_566 1_565
Se3 La4 V1 46.40(2) . 1_565
Se1 La4 V1 163.26(4) 1_655 1_565
Se1 La4 V1 106.757(19) . 1_565
Se3 La4 V1 89.14(2) 13_566 1_565
Se3 La4 V1 128.36(3) 13_666 1_565
V1 La4 V1 65.940(15) 1_665 1_565
O3 La4 La3 36.21(11) . 1_665
O2 La4 La3 41.0(2) 9_666 1_665
O2 La4 La3 97.2(2) 9_566 1_665
Se3 La4 La3 104.20(3) . 1_665
Se1 La4 La3 69.91(3) 1_655 1_665
Se1 La4 La3 107.65(3) . 1_665
Se3 La4 La3 171.92(3) 13_566 1_665
Se3 La4 La3 112.078(17) 13_666 1_665
V1 La4 La3 59.596(16) 1_665 1_665
V1 La4 La3 93.80(2) 1_565 1_665
O3 La4 La3 36.21(11) . 1_565
O2 La4 La3 97.2(2) 9_666 1_565
O2 La4 La3 41.0(2) 9_566 1_565
Se3 La4 La3 104.20(3) . 1_565
Se1 La4 La3 107.65(3) 1_655 1_565
Se1 La4 La3 69.91(3) . 1_565
Se3 La4 La3 112.078(17) 13_566 1_565
Se3 La4 La3 171.92(3) 13_666 1_565
V1 La4 La3 93.80(2) 1_665 1_565
V1 La4 La3 59.596(16) 1_565 1_565
La3 La4 La3 63.45(2) 1_665 1_565
La3 Se1 La3 77.33(4) 5_455 5
La3 Se1 La2 98.22(2) 5_455 1_455
La3 Se1 La2 156.06(6) 5 1_455
La3 Se1 La2 156.05(6) 5_455 .
La3 Se1 La2 98.22(2) 5 .
La2 Se1 La2 76.20(4) 1_455 .
La3 Se1 La4 123.24(5) 5_455 .
La3 Se1 La4 77.28(3) 5 .
La2 Se1 La4 122.85(5) 1_455 .
La2 Se1 La4 77.51(3) . .
La3 Se1 La4 77.28(3) 5_455 1_455
La3 Se1 La4 123.24(5) 5 1_455
La2 Se1 La4 77.51(3) 1_455 1_455
La2 Se1 La4 122.86(5) . 1_455
La4 Se1 La4 75.89(4) . 1_455
La1 Se2 La1 78.74(6) . 1_655
La1 Se2 La2 139.13(3) . 5_545
La1 Se2 La2 88.52(2) 1_655 5_545
La1 Se2 La2 88.52(2) . 14_446
La1 Se2 La2 139.13(3) 1_655 14_446
La2 Se2 La2 123.63(7) 5_545 14_446
La1 Se2 La2 139.13(3) . 14_546
La1 Se2 La2 88.52(2) 1_655 14_546
La2 Se2 La2 78.10(4) 5_545 14_546
La2 Se2 La2 76.12(3) 14_446 14_546
La1 Se2 La2 88.52(2) . 5_445
La1 Se2 La2 139.13(3) 1_655 5_445
La2 Se2 La2 76.12(3) 5_545 5_445
La2 Se2 La2 78.10(4) 14_446 5_445
La2 Se2 La2 123.63(7) 14_546 5_445
V1 Se3 V1 94.58(5) 1_665 1_565
V1 Se3 La4 77.90(3) 1_665 .
V1 Se3 La4 77.90(3) 1_565 .
V1 Se3 La4 166.37(5) 1_665 13_566
V1 Se3 La4 96.522(13) 1_565 13_566
La4 Se3 La4 96.74(4) . 13_566
V1 Se3 La4 96.522(13) 1_665 13_666
V1 Se3 La4 166.37(5) 1_565 13_666
La4 Se3 La4 96.74(4) . 13_666
La4 Se3 La4 71.47(3) 13_566 13_666
V1 Se3 La3 71.42(2) 1_665 9_666
V1 Se3 La3 120.71(5) 1_565 9_666
La4 Se3 La3 144.814(18) . 9_666
La4 Se3 La3 109.11(4) 13_566 9_666
La4 Se3 La3 70.63(3) 13_666 9_666
V1 Se3 La3 120.71(5) 1_665 9_566
V1 Se3 La3 71.42(2) 1_565 9_566
La4 Se3 La3 144.814(18) . 9_566
La4 Se3 La3 70.63(3) 13_566 9_566
La4 Se3 La3 109.11(4) 13_666 9_566
La3 Se3 La3 68.70(3) 9_666 9_566
O2 V1 O2 180.0 9_556 .
O2 V1 Se3 90.47(19) 9_556 9_666
O2 V1 Se3 89.53(19) . 9_666
O2 V1 Se3 89.53(19) 9_556 1_445
O2 V1 Se3 90.47(19) . 1_445
Se3 V1 Se3 180.0 9_666 1_445
O2 V1 Se3 90.47(19) 9_556 9_566
O2 V1 Se3 89.53(19) . 9_566
Se3 V1 Se3 94.58(5) 9_666 9_566
Se3 V1 Se3 85.42(5) 1_445 9_566
O2 V1 Se3 89.53(19) 9_556 1_545
O2 V1 Se3 90.47(19) . 1_545
Se3 V1 Se3 85.42(5) 9_666 1_545
Se3 V1 Se3 94.58(5) 1_445 1_545
Se3 V1 Se3 180.00(6) 9_566 1_545
O2 V1 La4 36.25(11) 9_556 1_445
O2 V1 La4 143.75(11) . 1_445
Se3 V1 La4 124.30(3) 9_666 1_445
Se3 V1 La4 55.70(3) 1_445 1_445
Se3 V1 La4 76.33(3) 9_566 1_445
Se3 V1 La4 103.67(3) 1_545 1_445
O2 V1 La4 143.75(11) 9_556 9_666
O2 V1 La4 36.25(11) . 9_666
Se3 V1 La4 55.70(3) 9_666 9_666
Se3 V1 La4 124.30(3) 1_445 9_666
Se3 V1 La4 103.67(3) 9_566 9_666
Se3 V1 La4 76.33(3) 1_545 9_666
La4 V1 La4 180.00(2) 1_445 9_666
O2 V1 La4 143.75(11) 9_556 9_566
O2 V1 La4 36.25(11) . 9_566
Se3 V1 La4 103.67(3) 9_666 9_566
Se3 V1 La4 76.33(3) 1_445 9_566
Se3 V1 La4 55.70(3) 9_566 9_566
Se3 V1 La4 124.30(3) 1_545 9_566
La4 V1 La4 114.059(15) 1_445 9_566
La4 V1 La4 65.941(15) 9_666 9_566
O2 V1 La4 36.25(11) 9_556 1_545
O2 V1 La4 143.75(11) . 1_545
Se3 V1 La4 76.33(3) 9_666 1_545
Se3 V1 La4 103.67(3) 1_445 1_545
Se3 V1 La4 124.30(3) 9_566 1_545
Se3 V1 La4 55.70(3) 1_545 1_545
La4 V1 La4 65.941(15) 1_445 1_545
La4 V1 La4 114.059(15) 9_666 1_545
La4 V1 La4 180.00(2) 9_566 1_545
La1 O1 La1 118.3(6) 1_665 1_565
La1 O1 La2 105.88(2) 1_665 .
La1 O1 La2 105.88(2) 1_565 .
La1 O1 La2 105.88(2) 1_665 10_556
La1 O1 La2 105.88(2) 1_565 10_556
La2 O1 La2 115.5(5) . 10_556
V1 O2 La4 114.6(3) . 9_666
V1 O2 La4 114.6(3) . 9_566
La4 O2 La4 113.6(4) 9_666 9_566
V1 O2 La3 110.4(4) . 9_556
La4 O2 La3 100.9(3) 9_666 9_556
La4 O2 La3 100.9(3) 9_566 9_556
La4 O3 La3 107.8(3) . 1_665
La4 O3 La3 107.8(3) . 1_565
La3 O3 La3 115.9(4) 1_665 1_565
La4 O3 La2 116.2(4) . .
La3 O3 La2 104.8(3) 1_665 .
La3 O3 La2 104.8(3) 1_565 .
La3 O4 La1 135.2(5) 1_565 1_565
La3 O4 La2 103.8(3) 1_565 1_455
La1 O4 La2 101.9(3) 1_565 1_455
La3 O4 La2 103.8(3) 1_565 .
La1 O4 La2 101.9(3) 1_565 .
La2 O4 La2 108.6(4) 1_455 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
La1 O1 2.322(7) 1_445
La1 O1 2.322(7) 1_545
La1 O4 2.407(10) 10_546
La1 O4 2.407(10) 1_545
La1 Se2 3.1419(19) 1_455
La1 Se2 3.1419(19) .
La1 La2 3.7745(11) 10_446
La1 La2 3.7745(11) 1_445
La1 La2 3.7745(11) 10_546
La1 La2 3.7745(11) 1_545
La1 La1 3.9859(2) 1_655
La1 La1 3.9859(2) 1_455
La2 O1 2.408(7) .
La2 O3 2.430(10) .
La2 O4 2.453(6) 1_655
La2 O4 2.453(6) .
La2 Se1 3.2300(13) .
La2 Se1 3.2300(13) 1_655
La2 Se2 3.2328(12) 5_455
La2 Se2 3.2328(12) 5
La2 La1 3.7745(11) 1_665
La2 La1 3.7745(11) 1_565
La2 La3 3.7869(10) 1_665
La2 La3 3.7869(10) 1_565
La3 O3 2.351(5) 1_445
La3 O3 2.351(5) 1_545
La3 O4 2.358(9) 1_545
La3 O2 2.533(10) 9_556
La3 Se1 3.1897(14) 5_545
La3 Se1 3.1897(14) 5_445
La3 Se3 3.5319(14) 9_666
La3 Se3 3.5319(14) 9_566
La3 La2 3.7868(10) 1_445
La3 La2 3.7868(10) 1_545
La3 La4 3.7900(11) 1_445
La3 La4 3.7900(11) 1_545
La4 O3 2.341(10) .
La4 O2 2.382(5) 9_666
La4 O2 2.382(5) 9_566
La4 Se3 3.0943(16) .
La4 Se1 3.2409(13) 1_655
La4 Se1 3.2410(13) .
La4 Se3 3.4126(14) 13_566
La4 Se3 3.4126(14) 13_666
La4 V1 3.6622(7) 1_665
La4 V1 3.6622(7) 1_565
La4 La3 3.7900(11) 1_665
La4 La3 3.7900(11) 1_565
Se1 La3 3.1898(14) 5_455
Se1 La3 3.1898(14) 5
Se1 La2 3.2299(13) 1_455
Se1 La4 3.2410(13) 1_455
Se2 La1 3.1419(19) 1_655
Se2 La2 3.2329(12) 5_545
Se2 La2 3.2329(12) 14_446
Se2 La2 3.2329(12) 14_546
Se2 La2 3.2329(12) 5_445
Se3 V1 2.7122(10) 1_665
Se3 V1 2.7122(10) 1_565
Se3 La4 3.4126(14) 13_566
Se3 La4 3.4126(14) 13_666
Se3 La3 3.5319(14) 9_666
Se3 La3 3.5319(14) 9_566
V1 O2 1.962(9) 9_556
V1 O2 1.963(9) .
V1 Se3 2.7122(10) 9_666
V1 Se3 2.7122(10) 1_445
V1 Se3 2.7122(10) 9_566
V1 Se3 2.7122(10) 1_545
V1 La4 3.6621(7) 1_445
V1 La4 3.6621(7) 9_666
V1 La4 3.6621(7) 9_566
V1 La4 3.6621(7) 1_545
O1 La1 2.322(7) 1_665
O1 La1 2.322(7) 1_565
O1 La2 2.408(7) 10_556
O2 La4 2.382(5) 9_666
O2 La4 2.382(5) 9_566
O2 La3 2.533(10) 9_556
O3 La3 2.351(5) 1_665
O3 La3 2.351(5) 1_565
O4 La3 2.358(9) 1_565
O4 La1 2.407(10) 1_565
O4 La2 2.453(6) 1_455
